|Organic-skinned inorganic nanoparticles: surface-confined polymerization of 6-(3-thienyl)hexanoic acid bound to nanocrystalline TiO2.|
|Jump to Full Text|
|PMID: 21888639 Owner: NLM Status: PubMed-not-MEDLINE|
|There are many practical difficulties in direct adsorption of polymers onto nanocrystalline inorganic oxide surface such as Al2O3 and TiO2 mainly due to the insolubility of polymers in solvents or polymer agglomeration during adsorption process. As an alternative approach to the direct polymer adsorption, we propose surface-bound polymerization of pre-adsorbed monomers. 6-(3-Thienyl)hexanoic acid (THA) was used as a monomer for poly[3-(5-carboxypentyl)thiophene-2,5-diyl] (PTHA). PTHA-coated nanocrystalline TiO2/FTO glass electrodes were prepared by immersing THA-adsorbed electrodes in FeCl3 oxidant solution. Characterization by ultraviolet/visible/infrared spectroscopy and thermal analysis showed that the monolayer of regiorandom-structured PTHA was successfully formed from intermolecular bonding between neighbored THA surface-bound to TiO2. The anchoring functional groups (-COOH) of the surface-crawling PTHA were completely utilized for strong bonding to the surface of TiO2.|
|Viswanathan S Saji; Yimhyun Jo; Hoi Ri Moon; Yongseok Jun; Hyun-Kon Song|
Related Documents :
|22009709 - Synthesis and characterization of injectable, thermosensitive, and biocompatible acellu...
22188399 - Two-photon absorption enhancement of polymer-templated porphyrin-based j-aggregates.
23857559 - Controlling the interaction of light with polymer semiconductors.
22026189 - Organometallic chemistry in non-classical environments.
22029329 - Chaotrope vs. kosmotrope: which one has lower friction?
22103219 - Fabrication and characterization of photoelectrode thin films with different morphologi...
17622159 - Relationship between swelling and the electrohydrodynamic properties of functionalized ...
22387039 - Label-free colorimetric sensor for ultrasensitive detection of heparin based on color q...
2111279 - Effect of metal chelators on thermoluminescence peaks of spinach chloroplasts and photo...
|Type: Journal Article Date: 2011-09-02|
|Title: Nanoscale research letters Volume: 6 ISSN: 1556-276X ISO Abbreviation: Nanoscale Res Lett Publication Date: 2011|
|Created Date: 2011-09-23 Completed Date: 2011-11-10 Revised Date: 2012-11-09|
Medline Journal Info:
|Nlm Unique ID: 101279750 Medline TA: Nanoscale Res Lett Country: United States|
|Languages: eng Pagination: 521 Citation Subset: -|
|i-School of Green Energy, UNIST, Ulsan 689-798, South Korea. firstname.lastname@example.org.|
|APA/MLA Format Download EndNote Download BibTex|
Journal ID (nlm-ta): Nanoscale Res Lett
Copyright ©2011 Saji et al; licensee Springer.
Received Day: 24 Month: 6 Year: 2011
Accepted Day: 2 Month: 9 Year: 2011
collection publication date: Year: 2011
Electronic publication date: Day: 2 Month: 9 Year: 2011
Volume: 6 Issue: 1
First Page: 521 Last Page: 521
Publisher Id: 1556-276X-6-521
PubMed Id: 21888639
|Organic-skinned inorganic nanoparticles: surface-confined polymerization of 6-(3-thienyl)hexanoic acid bound to nanocrystalline TiO2|
|Viswanathan S Saji1||Email: email@example.com|
|Yimhyun Jo1||Email: firstname.lastname@example.org|
|Hoi Ri Moon1||Email: email@example.com|
|Yongseok Jun1||Email: firstname.lastname@example.org|
|Hyun-Kon Song1||Email: email@example.com|
1i-School of Green Energy, UNIST, Ulsan 689-798, South Korea
Conducting polymers have attracted widespread academic and industrial research interest in the last two decades because of their potential applications in various fields such as light-emitting diodes, electrochromic devices, photovoltaic cells, anti-corrosion coatings, sensors, batteries, and supercapacitors [1-3]. Polythiophenes are one of the most widely studied conjugated conducting polymers due to their electrical properties, stability in doped and undoped states, nonlinear optical properties, and highly reversible redox switching [4,5]. Thiophene derivatives can be polymerized chemically, photochemically, or electrochemically to the corresponding oligothiophenes or polythiophenes [6-8]. However, poor processability of polythiophenes caused by their low solubility in solvents has impeded their practical applications. Even after grafting flexible hydrocarbon chains onto the polymer backbone, their solubility in most of organic solvents and water is too low. Despite the intensive research efforts for developing highly soluble and easily processable polythiophenes, yields of soluble polythiophenes were extremely low and/or synthetic processes demanded high costs and use of toxic solvents [9,10].
Oligothiophenes and polythiophenes have strong potentials in solar cell applications, functioning as a donor material in bulk heterojunction solar cells, as a hole-transporting layer in solid-state dye-sensitized solar cells (DSSCs) and as a light-absorbing species that injects electrons into the conduction band of n-type semiconductor (e.g., TiO2) in DSSCs [11,12]. Especially in the third cases, infiltrating sufficient amount of polymer into porous void of the nanostructured metal oxide electrodes is critical in obtaining high efficiency of polymeric-dye-based DSSCs. The cell performances are limited by the poor penetration of polymers into the porous nanocrystalline TiO2 network. Also, polymer aggregation within a void of porous electrodes can cause problems.
Instead of infiltrating pre-synthesized polymers, in situ formation of oligothiophenes or polythiophenes within nanostructured architectures would be one of the possible alternative ways to overcome the obstacles (low solubility, difficult infiltration into porous structure, and polymer aggregation). Several different polymerization strategies can be considered as the in situ formation of polymer. Electropolymerization of monomers would enable the in situ polymerization only if the substrate in which polymer is formed were conductive. High vacuum techniques including laser-induced vapor deposition; plasma polymerization; and × ray-, electron-, and ion-induced synthesis result in fragmentation of the monomer structure leading to defective incorporation into a target substrate . Photochemical and chemical polymerization [14,15] in a solution phase led to a successful deposition of polythiophenes onto nanostructured TiO2 electrodes. Zhang et al.  grafted poly(3-hexylthiophene) or P3HT chemically on a modified surface of TiO2 nanotubes. The polymerization was initiated from the monolayered 3HT-containing molecules covalently bound to TiO2. Fe3+ was used as an oxidizing agent to proceed polymerization in presence of the monomer 3HT. Tepavcevic et al.  polymerized 2,5-diiodothiophene (DIT) as monomer precursor on the surface of TiO2 nanotubes photochemically by ultraviolet irradiation. A thienyl radical and iodine atoms dissociated from DIT by UV absorption were preferentially adsorbed on TiO2 surface, forming initiation sites for polymerization. The reason for the surface specificity is that TiO2 serves as the primary conduit for transferring light energy. The photochemical and chemical polymerization can be classified as the surface-initiated polymerization in which direction of polymer growth was out of plane of target substrate.
In this context, it would be interesting to investigate whether polymerization is possible not between adsorbed monomers and free monomers in a solvent but between adsorbed ones. The surface-bound polymerization would lead to polymeric growth in a direction parallel to surface, forming a consecutively side-by-side bonded monolayer (Figure 1). In this work, therefore, we investigated a model system as the representative surface-bound polymerization. Carboxyl-functionalized thiophene monomer was adsorbed onto surface of nanocrystalline TiO2 electrodes. The -COOH groups facilitates strong linking of monomers onto TiO2. After removing extra free or loosely bound monomers from the TiO2 surface, the surface-bound monomers were polymerized in absence of free monomers in solution by using Fe3+ as an oxidant.
A commercial paste including TiO2 nanoparticles (T20, Solaronix, Switzerland) was coated on fluorine-doped tin oxide glass plates (SnO2:F, FTO) by a doctor blade and then sintered at 450°C for 30 min in a muffle furnace. The thickness of sintered films was estimated at approximately 10 μm by a surface profilometer.
A typical procedure of surface-bound polymerization is described as follows. The TiO2-coated electrodes were heated at 120°C for 10 min. After being cooled down to a specific temperature between room temperature and 80°C, the electrodes were immersed in a 20 mM monomer solution in acetonitrile for 24 h. 6-(3-Thienyl)hexanoic acid (THA, #4132, Rieke Metals, USA) was used as the monomer that is adsorbed on the immersion step. After the THA-adsorbed electrodes were rinsed thoroughly by acetonitrile and dried in air, they were dipped into a 10 mM FeCl3 solution in acetonitrile and kept stagnant during a specific time period. Then, the resultant polymer-adsorbed electrodes were washed repeatedly in copious amount of 1:1 mixture of methanol and ethanol to remove loosely bound species including polymers and ferric or ferrous ions.
As a control to the polymer-adsorbed TiO2 electrodes obtained by polymerizing the surface-bound THA, poly[3-(5-carboxypentyl)thiophene-2,5-diyl] (PTHA, Rieke 4032) was directly adsorbed on the same TiO2 electrodes. TiO2 electrodes were immersed in a 20 mM solution of PTHA in acetonitrile for 24 h. The immersion temperature was fixed at 80°C since the solubility of PTHA in acetonitrile is very low at room temperature. After the polymer adsorption, electrodes were repeatedly washed in acetonitrile to remove any loosely bound species.
The PTHA-adsorbed electrodes prepared from the surface-bound polymerization or direct adsorption were characterized by ultraviolet-visible spectroscopy (UV-vis, 2401PC, Shimadzu, Japan), Fourier-transformed infrared spectroscopy (FTIR, Varian 670, Varian, USA), and thermogravimetric analysis (TGA, TA SDT Q600; with a nitrogen atmosphere, TA instruments, USA).
Growth of PTHA or oligo-THA via surface-bound polymerization was traced by UV-vis absorption. Figure 2 shows the absorption spectra of PTHA or oligo-THA obtained by polymerizing surface-bound THA on TiO2 electrodes at different conditions of polymerization temperature and time. For a comparison, the spectrum of PTHA adsorbed on the same porous TiO2 electrode at 80°C for 1 day is also shown. A bare TiO2 electrode was employed as the reference. Typically, polythiophenes exhibit absorption maximum around 500 nm with an extended absorption tail reaching up to 650 nm . The absorption peak of oligomer or polymer obtained by surface-bound polymerization was observed at ~350 nm (Figure 2a) at room temperature. Its long tail extending up to 600 nm indicates some degree of oligomer/polymer formation. By increasing polymerization temperature (even with a shorter reaction time), the absorption peak gradually shifted to longer wavelength region or red color region (from 350 nm (a) through 400 nm (b) to 415 nm (c) in Figure 2). Simultaneously, the color of electrodes changed apparently from yellow through orange to dark red (the inset in Figure 2). The broad absorption in the range of 350 to 700 nm with strong absorbance (Figure 2c) guarantees significant formation of oligo/polythiophenes. As absorption is directly related to the polymer π conjugation length, it can be presumed that significant oligomerization or polymerization proceeded at higher temperature and longer reaction time. This is attributed to enhanced mobility of the adsorbed monomers and accelerated oxidation kinetics of monomers at higher temperatures which might have facilitated polymerization of adjacent thiophenes in the monolayer.
For comparison, the control sample obtained by polymer adsorption (Figure 2d) shows higher peak wavelength at 450 nm with lower intensity (versus Figure 2c), demonstrating more bright red color. Considering that the used PTHA for polymer adsorption is highly regioregular (98.5% or higher), the blue-shifted spectrum for surface-bound polymerization is related to a structure-less monolayer of PTHA of regiorandom geometry in nature with shorter conjugation lengths . In the conventional FeCl3-based polymerization of substituted thiophenes, polymerization happens through either 2- or 5-position of adjacent five-membered monomers. When a monomer is incorporated in a growing polymer chain, it can be added either with its head (2-position) or tail (5-position), resulting in three different possible couplings . The propagation is believed to be initiated by a thiophene radical cation. Then, the propagation proceeds through a carbocation since polymer chain cannot be neutral under the strong oxidizing conditions . In electrochemical polymerization, on the other hand, the oxidation of monomers produces a radical cation which can then be coupled with a next radical cation to form a di-cation dimer. The process repeats and hence the polymer chain grows . Tepavcevic et al. reported that UV irradiation caused the C-I bond of adsorbed monomers (2,5-diiodothiophene) to be selectively photodissociated and then produced monomer radicals with intact π ring structure that further coupled to oligothiophenes/polythiophenes molecules . In the present case, the functional group of PTHA is strongly bonded to the TiO2 surface. As soon as the electrodes were dipped in the oxidant solution, a radical cation is formed in each monomer. Due to the geometric restriction of surface-bound configuration, propagation proceeds between adjacent adsorbed monomers. Also, with the same reason, regiorandom structure is preferred with a limited degree of polymerization.
FTIR spectra were compared between PTHAs prepared by surface-bound polymerization and direct adsorption on TiO2 (Figure 3a). Qualitatively similar spectra were obtained from both samples, consistent with that of polythiophenes . The surface-bound polymerization showed lower intensities of the peaks corresponding to aliphatic and aromatic C-H stretching (2,850 and 2,930 cm-1), compared with polymer adsorption. It indicates that smaller amount of PTHA is obtained or degree of polymerization is limited with surface-bound polymerization. This is easily understandable since the amount of monomers and the intermolecular collision between surface-bound monomers cannot help being limited. Both of PTHA have the similar intensity of peaks centered at 1,380 and 1,630 cm-1 ascribed to the symmetric and anti-symmetric stretch modes of the carboxylate group . Monomer molecules (THA) for surface-bound polymerization would be adsorbed at full coverage over TiO2 if the whole adsorption sites of TiO2 surface are occupied by polymer PTHA for polymer adsorption as the control. However, the peak at 1,720 cm-1 attributed to free carboxylic acid group (indicated by arrow in Figure 3a) is observed only with PTHA prepared by polymer adsorption. There exist free -COOH groups in the polymer backbone which are not strongly bound to TiO2 surface. The clear absence of the peak with surface-bound polymerization supports all of the carboxylate functional group is completely used for bonding to TiO2 surface. In other words, all of the -COOH groups in a polymer backbone does not necessarily get involved in adsorption process of direct polymer adsorption.
To support conclusions from FTIR spectra, mass change was investigated with temperature by TGA (Figure 3b). Samples were obtained by scratching PTHA-coated TiO2 electrodes prepared by surface-bound polymerization and polymer adsorption. The weight percent (m%) was calculated by: m% = (m -m700)/(m110 -m700) with m = mass at a certain temperature, m700 and m110 = mass at 700°C and 110°C. Since TiO2 is stable within the temperature range examined, PTHA is wholly responsible for the weight loss. Three regions of degradation processes were clearly shown for both of PTHA [22,23]:
1. Small molecule decomposition region (up to T1 indicated by circle in Figure 3b, T1 = 430°C for surface-bound polymerization and 490°C for polymer adsorption): ascribed to loss of doped molecules or pendanted molecular structure including Cl-as a dopant, functional groups, and a small fraction of thiophene;
2. Thermally stable region (between T1 and T2);
3. Polymer degradation region (from T2 indicated by double circle in Figure 3b): oxidative degradation of polymer backbone.
Even if characteristic polymer decomposition looks similar in both cases at the first look, a closer analysis of the thermograms leads to the conclusion that is obtained above from FTIR: smaller amount of PTHA or lower degree of polymerization with surface-bound polymerization. Lower T1 indicates the smaller amount of PTHA formed on surface while the abrupt decrease of mass after T2 in the region (3) is due to the low degree of polymerization.
We showed that specifically surface-crawling polymer can be developed by polymerizing its corresponding monomers surface-bound to metal oxide nanoparticles. As a model of the organic/inorganic hybrid system, TiO2 and THA were chosen as the inorganic nano-substrate and the organic monomer that will be polymerized into PTHA, respectively. All of the anchoring functional groups (-COOH) were completely used for connecting polymer backbone to the surface of TiO2, while free carboxylates not participating in bonding were observed with direct polymer adsorption on TiO2. Degree of oligomerization/polymerization or the total amount of PTHA was limited by the geometric restriction of the surface-bound THA. Although the polymers obtained by this method may have lower regioregularity and π conjugation, the specifically surface-confined polymerization would be of a reference methodology for basic studies of completely surface-bonded polymer films and for developing hybrid solar cells and organic electronics.
The authors declare that they have no competing interests.
VSS proposed the original idea, carried out most of experiments including synthesis and analysis and wrote the first draft of manuscript. YJ analyzed material properties. HRM and YJ detailed the original idea and modified the first draft of manuscript. HKS designed and coordinated the whole work and finalized the manuscript. All authors read and approved the final manuscript.
This work was supported by NRF Korea (New Faculty/2009-0063811, WCU/R31-2008-000-20012-0 and 2010-0029321).
|Shirakawa H,Louis EJ,Macdiarmid AG,Chiang CK,Heeger AJ,Synthesis of electrically conducting organic polymers - halogen derivatives of polyacetylene, (CH)xJournal of the Chemical Society-Chemical CommunicationsYear: 1977578580|
|Reddinger JL,Reynolds JR,Molecular engineering of pi-conjugated polymersAdvances in Polymer ScienceYear: 19991455712210.1007/3-540-70733-6_2|
|Brotherston ID,Mudigonda DSK,Osborn JM,Belk J,Chen J,Loveday DC,Boehme JL,Ferraris JP,Meeker DL,Tailoring the electrochromic properties of devices via polymer blends, copolymers, laminates and patternsElectrochimica ActaYear: 1999442993300410.1016/S0013-4686(99)00014-6|
|Roncali J,Yassar A,Garnier F,Highly conducting thin-films of polythiophenesJournal De Chimie Physique Et De Physico-Chimie BiologiqueYear: 1989868592|
|Patil AO,Heeger AJ,Wudl F,Optical-properties of conducting polymersChemical ReviewsYear: 19888818320010.1021/cr00083a009|
|Englebienne P,Weiland M,Synthesis of water-soluble carboxylic and acetic acid-substituted poly(thiophenes) and the application of their photochemical properties in homogeneous competitive immunoassaysChemical CommunicationsYear: 199616511652|
|Piletsky SA,Piletska EV,Karim K,Davis F,Higson SPJ,Turner APF,Photochemical polymerization of thiophene derivatives in aqueous solutionChemical CommunicationsYear: 200422222223|
|Li GT,Kossmehl G,Welzel HP,Engelmann G,Hunnius WD,Plieth W,Zhu HS,Reactive groups on polymer coated electrodes, 7 new electrogenerated electroactive polythiophenes with different protected carboxyl groupsMacromolecular Chemistry and PhysicsYear: 199819952553310.1002/(SICI)1521-3935(19980401)199:4<525::AID-MACP525>3.0.CO;2-9|
|Iarossi D,Mucci A,Schenetti L,Seeber R,Goldoni F,Polymerization and characterization of 4, 4'-bis(alkylsulfanyl)-2, 2'-bithiophenesMacromoleculesYear: 1999321390139710.1021/ma9813340|
|Chayer M,Faid K,Leclerc M,Highly conducting water-soluble polythiophene derivativesChemistry of MaterialsYear: 199792902290510.1021/cm970238v|
|Oregan B,Gratzel M,A low-cost, high-efficiency solar-cell based on dye-sensitized colloidal TiO2 filmsNatureYear: 199135373774010.1038/353737a0|
|Brabec CJ,Sariciftci NS,Hummelen JC,Plastic solar cellsAdvanced Functional MaterialsYear: 200111152610.1002/1616-3028(200102)11:1<15::AID-ADFM15>3.0.CO;2-A|
|Natarajan S,Kim SH,Photochemical conversion of 2,5-diiodothiophene condensed on substrates to oligothiophene and polythiophene thin films and micro-patternsThin Solid FilmsYear: 200649660661110.1016/j.tsf.2005.09.098|
|Zhang Y,Wang CW,Rothberg L,Ng MK,Surface-initiated growth of conjugated polymers for functionalization of electronically active nanoporous networks: synthesis, structure and optical propertiesJournal of Materials ChemistryYear: 2006163721372510.1039/b605421h|
|Tepavcevic S,Darling SB,Dimitrijevic NM,Rajh T,Sibener SJ,Improved hybrid solar cells via in situ UV polymerizationSmallYear: 200951776178310.1002/smll.20090009319367599|
|Kim YG,Kim JH,Ahn HJ,Kang BW,Sung CM,Samuelson LA,Kumar J,Molecular assembly by sequential ionic adsorption of nanocrystalline TiO2 and a conjugated polymerJournal of Macromolecular Science-Pure and Applied ChemistryYear: 2003A4013071316|
|Leclerc M,Diaz FM,Wegner G,Structural-analysis of poly(3-alkylthiophene)sMakromolekulare Chemie-Macromolecular Chemistry and PhysicsYear: 198919031053116|
|Andersson MR,Selse D,Berggren M,Jarvinen H,Hjertberg T,Inganas O,Wennerstrom O,Osterholm JE,Regioselective polymerization of 3-(4-octylphenyl)thiophene with FeCl3MacromoleculesYear: 1994276503650610.1021/ma00100a039|
|Lukkari J,Alanko M,Pitkanen V,Kleemola K,Kankare J,Photocurrent spectroscopic study of the initiation and growth of poly(3-methylthiophene) films on electrode surfaces with different adsorption propertiesJournal of Physical ChemistryYear: 1994988525853510.1021/j100085a036|
|Yanagida S,Senadeera GKR,Nakamura K,Kitamura T,Wada Y,Polythiophene-sensitized TiO2 solar cellsJournal of Photochemistry and Photobiology a-ChemistryYear: 2004166758010.1016/j.jphotochem.2004.04.039|
|Duffy NW,Dobson KD,Gordon KC,Robinson BH,McQuillan AJ,In situ infrared spectroscopic analysis of the adsorption of ruthenium(II) bipyridyl dicarboxylic acid photosensitisers to TiO2 in aqueous solutionsChemical Physics LettersYear: 199726645145510.1016/S0009-2614(97)00035-3|
|Hacaloglu J,Yigit S,Akbulut U,Toppare L,Thermal degradation of polythiophene natural rubber and polythiophene synthetic rubber conducting polymer compositesPolymerYear: 1997385119512410.1016/S0032-3861(97)00056-6|
|Mohammad F,Calvert PD,Billingham NC,Thermal stability of electrochemically prepared polythiophene and polypyrroleBulletin of Materials ScienceYear: 19951825526110.1007/BF02749663|
Keywords: surface-bound polymerization, nanocrystalline TiO2, thiophenes, FeCl3.
Previous Document: Reexpansion pulmonary edema following a posttraumatic pneumothorax: a case report and review of the ...
Next Document: Solid-phase molecular recognition of cytosine based on proton-transfer reaction. Part II. supramolec...